Modeling of Phase Transformation
Embed Size (px)
Transcript of Modeling of Phase Transformation
2008-09MODELING OF PHASE TRANSFORMATION KINETICS OF PLAIN CARBON STEELA THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENT FOR THE DEGREE OF
Bachelor of Technology in Metallurgical and Materials Engineering By ANIRUDDHA CHATTERJEE & BISWARANJAN DASH
Department of Metallurgical and Materials Engineering National Institute of Technology Rourkela
MODELING OF PHASE TRANSFORMATION KINETICS OF PLAIN CARBON STEELA THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENT FOR THE DEGREE OF
Bachelor of Technology in Metallurgical and Materials Engineering By ANIRUDDHA CHATTERJEE & BISWARANJAN DASH Under the Guidance of
Department of Metallurgical and Materials Engineering National Institute of Technology Rourkela
Acknowledgement.With a great pleasure I would like to express my deep sense of gratitude to my project guide, Dr. B.C. Ray, Professor, Department of Metallurgy and Materials Engg., N.I.T. Rourkela, to undertake this particular project. I would also like to express my respect for his illuminating criticism throughout the project work. I would like to express my sincere gratitude to Prof A.K Panda, Professor and Coordinator, Department of Metallurgy and Materials Eng, N.I.T Rourkela, for his unselfish help and guidance at every stage of the project work and important information regarding the preparation of the report for this work. I also wish to thank the library (Information and Documentation Centre) staff for their help during the project work. I would like to thank my project partner Biswaranjan Dash for his constant support and help for the project work throughout the semester. I would also like to thank all of my colleagues and the faculty members of the Department of Metallurgy and Materials Engg., for their sincere cooperation and support throughout my project work till date. Last but not the least I am especially indebted to my parents for their constant support and belief that has made my project work till date successful.
Department of Metallurgy and Materials Engg.. N.I.T Rourkela, May 12th, 2009
Aniruddha Chatterjee Roll No-10504031, 8th Semester. B.Tech-Part (IV)
ABSTRACT.A mathematical model have been generated which incorporates the concept of isothermal/isokinetic steps in close association with the cooling curve to predict the transformation kinetics under continuous cooling conditions. Transformation kinetics under actual cooling conditions was predicted by the dilatometric analysis of the 1080 steel samples. The continuous cooling experiments were conducted for cooling rates of 5, 10, 15, 200 K/min to determine the time and temperature for start and end of pearlitic transformation respectively. The isothermal transformation data was also incorporated in the mathematical model to predict the continuous cooling transformation kinetics. The results of the mathematical model agree closely and in a similar manner with the measurements made at the four cooling rates.
2. THEORY...3 2.1 Austenite PearliteTransformation...........................................3 2.2 Transformation Mechanism.....3 2.2.1 Hull-Mehl Model.........................4 2.3 Nucleation and Growth5 2.4 Factors affecting Pearlitic Transformation..15 2.4.1 Austenitic Grain size..........................15 188.8.131.52 Effect on Pearlitic nodule size..15 184.108.40.206 Effect on Pearlitic colony size..15 220.127.116.11 Effect on Interlamellar spacing16 2.4.2 Cooling Rate..16 18.104.22.168 Effect on Interlamellar spacing.......16 22.214.171.124 Effect on Pearlitic colony size.17 2.5 Time-Temperature-Transformation curves..18 2.6 Continuous Cooling Transformations21 2.6.1. Additivity Rule and CCT Kinetics.23 2.6.2. Conditions for Transformed Fractions to be Additive24. 2.6.3. The Non isothermal Rate laws for isokinetic reactions..26 2.7Effect of Deformation on Transformation kinetics27 2.7.1 Determination of Incubation period..28.
4. EXPERMENTAL WORK..36
4.1 Dilatometric analysis36
5. RESULTS AND DISCUSSION 38
7. SCOPE FOR FUTURE WORK.48
1. INTRODUCTION.The steel industry is rapidly adopting continuous processes including continuous casting, continuous annealing and continuous heat treatment to minimize production costs, to save time and to improve product quality. The prediction of phase transformations in heat-treatment processes such as controlled cooling of wire rod is made difficult by the complex nature of coupled heat transfer and phase transformation kinetics. Heat transfer at the surface of the metal, for example, depends upon local cooling conditions which change with temperature, fluid properties and relative fluid velocity. Within the metal, the thermo-physical properties changes with temperature and the heat of transformation is released. The factors which affect transformation kinetics are cooling rate, prior-austenitic grain size, and steel composition. Thus, the
problem of transformation kinetics under non-isothermal conditions is of tremendous practical importance. However, experimental and theoretical aspects of the
decomposition are most conveniently studied isothermally. So it is desirable to relate the transformation behavior of steel under continuous cooling with its isothermal transformation data. The isothermal transformation diagram is a valuable tool for studying the temperature dependence of austenitic transformations. Information of a very important and practical nature can be obtained from a series of isothermal reaction curves determined at a number of temperatures. Even in a single, such as austenite to pearlite transformation, the product varies in appearance with the transformation temperature. The simplest one is the TTT curve for eutectoid steel. From this plot, the time required to start the transformation and the time required to complete the transformation may be obtained. This is done in practice by observing the time to get a finite amount of transformation product, usually 1 percent, corresponding to the start of the transformation. The end of the transformation is then arbitrarily taken as the time to transform 99 percent of the austenite to pearlite. On the other hand a continuous cooling transformation curve gives us idea about austenitic transformations under continuous cooling conditions i.e. transformation kinetics under different cooling rates. Since most of the transformations occur in continuous cooling conditions, CCT curves are more of importance than the TTT curves.
The picture becomes clearer if we superimpose different cooling rates upon the CCT curve to identify the time to start transformation i.e. 1 percent of transformation product and time to end transformation, usually 99 percent of transformation product. There have been several attempts to predict the cooling transformation from an experimentally determined set of isothermal transformation curves. The initial work in this direction was carried out by Prakash K.Aggarwal and J.K. Brimacombe (1) whose model consists of heat flow equations and transient distribution of temperature and fraction transformed can be predicted simultaneously. Scheil, (2) and later Steinberg, (3) presented an additivity rule for calculating the temperature at which transformation begins during continuous cooling. An additive reaction implies that the total time to reach a specified stage of transformation is by addition of fraction of time to reach this stage isothermally until the sum reaches unity. Most of the previous studies have been limited to the beginning of the transformation and not many work (4-7) have been carried out about the continuous cooling transformation over the entire range of reactions. In the present work an attempt will be made to model the transformation kinetics for austenite to pearlite transformation for 1080 eutectoid steel under continuous cooling conditions using the isothermal transformation data. Apart from that prediction of continuous cooling transformation kinetics will be carried out under the effect of factors such as prior-austenitic grain size, deformation, cooling rates etc.
2. THEORY.2.1 Austenite Pearlite Transformation.The most famous and commercially important transformation occurs at 0.77%wt C known as eutectoid transformation. Today fully pearlitic steels are of great importance in a number of extremely demanding structural applications. Fully pearlitic carbon steels are used in a number of important applications where high strength, wear resistance, ductility, toughness, and low cost are important. Chief among such applications are high-strength wires and high-strength tee rails. When eutectoid steel is heated to the austenising temperature and held there for a sufficient time, the structure will become homogenous austenite. On very slow cooling under conditions approaching equilibrium, the structure will remain that of austenite until just above the eutectoid temperature .At the eutectoid temperature or just below it, the entire structure of austenite will transform into a lamellar product called pearlite which consists of alternate layers of ferrite and cementite. The region in which ferrite and cementite plates are parallel to one another is called a colony. However, different pearlite colonies have different lamellar orientation, and, as the transformation progresses, neighboring colonies join together and continue to advance into the austenite, such that when transformation occurs at lower degrees of undercooling, the colony groups advance in a roughly spherical boundary leading to the formation of a nodule.
2.2 Transformation Mechanism.Pearlite is a lamellar product of eutectoid decomposition which can form in steels during transformation under isothermal, continuous-cooling, or forced velocity (8, 9) (directional) gr